Effect of Plasticizer on Oxygen Permeability of Cast Polylactic Acid (PLA) Films Determined Using Dynamic Accumulation Method
Effect of Plasticizer on Oxygen Permeability of
Cast Polylactic Acid (PLA) Films Determined
Using Dynamic Accumulation Method
Kurniawan Yuniarto Hadi Karia Purwadaria
Bogor Agricultural University Swiss-German University
Bruce A. Welt Ayman Abdellatief
University of Florida University of Florida
Y Aris Purwanto Titi C. Sunarti
Bogor Agricultural University Bogor Agricultural University
National Nuclear Energy Agency, Indonesia
Polylactic acid (PLA) is becoming an increasingly important biopolymer for packaging applications. PLA
brittleness limits its applicability. This study evaluated PLA properties with increasing amounts of addedpolyethylene glycol (PEG) plasticizer. Oxygen transmission rate (OTR) of cast films was determined us- ing the newly available Dynamic Accumulation (DA) method. Arrhenius temperature sensitivity of OTR and polymer Permeability was also determined. Permeability of neat PLA is 4.848 ml mm (STP)/m2 s
kPa; hence, 4.84 ml mm (STP)/m2 s kPa, 4.07 ml mm (STP)/m2 s kPa and 5.42 ml mm (STP)/m2 s kPa byadding PEG 1 %, 5% and 10% respectively. The main conclusion from this work is increasing PEG will
enhance the PLA permeability number but excess PEG in PLA film will decrease the permeability number.
KEYWORDS: OTR, oxygen transmission rate, dynamic accumulation, PLA, polylactic acid This work was supported in part by the University of Florida, Agricultural Experiment Stations at the Agricultural and Biological Engineering Department’s Packaging Engineering Laboratory and Directorate General of Higher Education (DGHE) Ministry of Education Republic of Indonesia.
Polylactic acid (PLA) is a thermoplastic bio-poly- ester polymer with properties similar to polystyre- nethat is also compostable under commercial com- posting conditions. To the extent that bio-based polymers offer actual or perceived environmental benefits, packaging manufacturers may be able to realize competitive advantage by incorporating bio-polymers into their products. Therefore, in- terest in PLA for plastic packaging applications is increasing. Currently, PLA is being commercialized and used as a food packaging polymer. However, PLA is known to be brittle, which limits its applicability. Therefore, plasticizers may be added to enhance ductility and flexibility of PLA based packaging. Plasticizers help to increase polymer chain mo- bility by decreasing intermolecular forces  and hydrogen bonding between polymer chains.[6,7] Plasticizers also affect glass transition temperature and gas permeability.
Oxygen barrier properties of PLA have been re- ported to be between polyethylene terephthalate and polystyrene.[8,9] A relatively low glass tran- sition temperature permits greater polymer chain mobility at moderate temperatures resulting in higher gas diffusivity and overall permeability. Knowledge of gas transmission properties of packaging materials are critical for a successful package design for many products. Perme- ation is influenced by solubility of permeant in the film, rate of diffusion of permeant through the film, film thickness, temperature and specific par- tial pressure difference. Oxygen transmission rate (OTR) is an important film specification parameter. Film and pack- age OTR are important for determining product shelf life. Until recently, the steady-state meth- od for measuring OTR, as described by ASTM D-3985, has been widely used. However, a new approach based on the principle of dynamic accumulation (DA) has been gaining popular- ity due to simplicity and relatively low cost. Briefly, DA involves mounting a film between an accumulation chamber and a test gas. For the case of measuring OTR via DA, the accumulation chamber is initially flushed with an inert gas such as nitrogen and the test gas is air or oxygen. Once the accumulation chamber is flushed, it is sealed and oxygen accumulation is monitored over time, typically with a non-destructive oxygen sensor such as those based on florescence quenching (e.g. Oxysense, Dallas, TX). A schematic of a typical DA permeation cell is depicted in Figure 1.
Figure 1. DA permeation cell.
The objective of this work was to measure OTR of cast PLA films with increasing concentrations of plasticizer and to obtain Arrhenius temperature sensitivity parameters of OTR for sample films.
2.0 MATERIAL AND METHOD
Polylactic acid pellets were purchased from Shen- zen Essu Industrial Co.Ltd.. Guangdong, China with molecular weight (M W ) ca. 100,000 g/mol. Chloroform C606-4 HPLC grade, was purchased from Fisher Scientific, USA. Polyethylene Gly- col-400 was purchased from Fisher Scientific, USA with average molecular weight 380-420, density 1.13 g/mol.
2.2. PLA FILM CASTING PREPARATION
PLA films were cast from 5% (w/v) weight solu- tion in chloroform using via casting in glass petri dishes. 20 gram PLA were dissolved in 400 ml chloroform and stirred vigorously for 30 minutes at 60oC. Then, PEG was added in concentrations of 0, 1, 5 and 10% (w/w), respectively.
To achieve different film thicknesses, PLA solu- tions were poured onto glass petridishes in vol- umes of 5, 10, 15 and 20 ml, respectively. Solu- tions were dried into films at 35oC for 15 hours. PLA film production were done in three replication each variable. Resultant PLA films were peeled from petri dishes and thicknesses were measured in 5 locations using a micrometer.
2.3. OTR MEASUREMENT
Dynamic accumulation experiments were per- formed using permeation cells and fluorescence oxygen detection equipment from Oxysense, Inc. (Model 310, Dallas, TX). The oxygen accumula- tion chamber had a sample area of 16.62 cm 2 and volume 8.3 cm 3 . Initially, the cell was purged with more than 10 volumes of industrial grade nitrogen from a compressed gas cylinder. Purging was fol- lowed by monitoring oxygen concentration de- crease to a constant zero level using the Oxysense Model 310 device. Industrial-grade oxygen (ap- proximately 100%) was used to purge the test-gas chamber. Oxygen concentration in the DA cham- ber was measured and recorded periodically using the Oxysense Model 310 (Oxysense, Inc). OTR was subsequently calculated as described by Ab- dellatief and Welt.  OTR measurements were performed at 15, 23 and 35oC using a fabricated bench top environmen- tal chamber equipped with feedback temperature controller. The system was comprised of a Peltier Effect mini-refrigerator (NuCool Model C-RNU- 281VS; Haier America Trading, LLC, NY, USA) and a 100 W light bulb controlled by a PID tem- perature controller (Omega Model CSC32; Omega Engineering, Inc., Stamford, CT, USA). The envi- ronmental chamber is capable of maintaining set point ±0.2 o
C. OTR measurement were replicated in three times.
3. RESULT AND DISCUSSION
3.1. OXYGEN TRANSMISSION RATE
OTR of the PLA films are plotted as a function of thickness (µm) (Figure 2). The OTR number de- crease with increasing film thickness. As expected, the film thickness has a role to reduce the PLA film OTR number. As expected, OTR is a function of film thickness.  OTR value of PLA films decrease with in- creasing of the thickness. As result, the OTR value is higher with a thinner of PLA films. The trend OTR of PLA films show exponentially. Exponen- tial equation prediction of PLA films OTR and thickness is 1640.7 e -0.012x .
OTR with initially increasing plasticizer is likely due to increased polymer crystallinity made possi- ble by the presence of plasticizer. Hence, the count of crystallinity intensity of PLA-PEG showed in- creasing by XRD analysis. The count of crystal- linity intensity neat PLA is 1500, otherwise PLA with addition PEG 1%, 5% and 10% are 1600, 2500 and 2000, respectively.
3.3. TEMPERATURE EFFECT Figure 2. OTR versus PLA film thickness (µm).
Decreasing OTR value of PLA films show a sig- nificance difference between 26 microns and 66 microns. OTR value reduced 2.4 times. Hence, PLA film thickness from 66 micron to 132 micron effected decreasing OTR value 1.6 times.
3.2. POLYETHYLENE GLYCOL EFFECT
Figure 4. Oxygen Transmission rate (OTR) value PLA film as function of thickness & temperature.
As expected, OTR increase with increasing tem- perature. The trend of decreasing OTR on PLA film among temperature treatment show a similar pattern. OTR of PLA films are plotted as a func- tion of temperature and thickness in Figure 4.
Figure 3. PEG concentration on OTR value. Related to the graph, the OTR trend is exponen-
tially among temperature gradient. Lower OTR number explain amount less oxygen is less to Plasticizer is commonly added to PLA to improve through pass the PLA film. As result, lower OTR flexibility and reduce brittleness. OTR of PLA number in PLA film shows a good barrier proper- films are plotted as a function of plasticizer (PEG) ties from oxygen penetration. It clears, tempera- concentration in Figure 3. ture 15oC result a best temperature condition of PLA film to prevent from oxygen permeation. En-
Addition of PEG plasticizer caused OTR to de- ergy activation of PLA film surrounding different crease up to plasticizer concentrations of about temperature in Figure 5. 5%, after which, OTR increased. The decrease in
OTR is a sample specific measurement. Using the thickness of the film and conditions of the test, OTR may be converted into a more general perme- ation coefficient, P ̅. Figure 6 shows P ̅ of PLA with increasing concentrations of plasticizer. As with Figure 3, a reduction in permeation coefficient at 5% plasticizer is likely due to increased crystallin- ity resulting from greater chain mobility. At 10% plasticizer, permeation coefficient increases. Per- meation coefficient of PLA film is also influenced by temperature. Arrhenius temperature sensitivity on permeation coefficient of PLA is shown in Fig-
Figure 5. Arrhenius temperature sensitivity param- ure 7. eters.
Activation Energy (Ea) of 23.869 kJ/mol and 7 pre-exponential factor (k ) of 5.243 x 10 .Fig 4. o Temperature effect on Oxygen Transmission rate (OTR) value as shown via Arrhenius Plot. The fol- lowing Arrhenius equation (Equation 1) can be used to predict OTR of this film at any absolute temperature (Kelvin):
3.3. PERMEABILITY Figure 7. Arrhenius temperature sensitivity on P ̅.
As expected, P ̅increased with increasing tem- perature. Figure 6 provides Arrhenius tempera- ture sensitivity parameters, Activation Energy (Ea) of 10.3kJ/mol and pre-exponential factor (k ) 4 o of 2.828 x 10 . The Ea for oxygen permeation is 8 4 closely 11.1 kJ/mol ) and below 28.4 kJ/mol ). Equation 2 can be used to estimate P ̅ at any abso- lute temperature (Kelvin).
Figure 6. PLA film PEG concentration on perme- ation coefficient.
4.0 CONCLUSIONS prepared by thermal and cold gelatinization
from non-conventional sources starches,” Oxygen barrier properties of PLA samples were Journal of Carbohydrate Polymer 2006, vol. actually improved up to about 5% PEG plasticizer. 60 (2), pp. 235-244,2006. Improvement in barrier properties were likely due  L. Bao, J.R. Dorgan, D. Knauss, S. Hait, to enhanced crystallization made possible by the N.S. Oliveira, and I.M. Marucho, “Gas presence of plasticizer. Beyond 5% plasticizer, permeation properties of ply (lactide acid) however, oxygen barrier properties decreased. revisited,” Journal of Membran Science,
As expected, OTR and permeability coefficients showed Arrhenius temperature sensitivity. Arrhe-  S. Mali, M.V.E. Grossmann, M.A. nius parameters were provided in order to permit Gracia,M.N. Martino, and N.E. Zaritzky, estimation of OTR or permeability coefficient of “Effects of controlled storage on thermal, cast PLA films at any temperature. mechanical and barrier properties of plasticized films from different starch
sources,” Journal of Food Engineering, vol.75 (4),pp. 453-460, 2006.  A.N. Frone, S. Berlioz, J-F. Chailan and  H.J. Lehermeier, and J.R. Dorgan, “Gas
D.M. Panaitescu,“Morphology and thermal permeation properties of poly (lactic acid),” properties of PLA-nanofibers composites,” Journal of Membran Science, vol. 190, pp.
Journal of Carbohydrate Polymer, vol. 91, (1) pp. 377-384, 2012.  A. Guinault, C. Sollogoub, V. Ducruet, and
 M.D. Sanchez-Garcia, E. Gimenez, J.M. S. Domenek, “Impact of crystallinity of Lagaron,“Morphology and barrier properties poly (lactide) on helium and oxygen barrier of solvent cast composites of thermoplastic properties,” European Polymer Journal, vol. biopolymers and purified cellulose fibers,” 48 (4), pp 779-788, 2012. Journal of Carbohydrate Polymers, vol.71,  S.C. George, andS. Thomas, “Transport phenomena through polymer system,” Prog.
 J.R. Dorgan,”Polylactide acid: Properties and prospects of an environmentally  Abdellatief A, Welt B. Comparison of benign plastic from renewable resources,” New Dynamic Accumulation Method for Macromol. Symp. 175, pp. 55-56, 2001 measuring oxygen transmission rate of
 R.Auras, G Kale, and S.P. Singh, packaging against the steady-state method “Degradation of commercial biodegradable described by ASTM D 3985 [J]. Journal of packages under real and ambient exposure Packaging Technol Sci, 2012, (12): 1-8. condition,” Journal of Polymer and  Valentina S, “Food packaging permeability Environtmental,vol. 14 (3), pp. 317-334, behaviour. A report [J]. Hindawi Publishing 2006.
Coorporation,” International Journal of  C.A. Romera-Bastida, L.A. Bello-Perez, Polymer Science, vol. 12, pp. 1-12, 2012
M.A. Garcia, M.N. Martino, J. Solorza-  American Society Test for Material, ASTM, Feria,andN.E. Zaritzky, “Physicochemical “D-3985 Standard test method for oxygen and microstructural characterization of films gas transmission rate through plastic film and sheeting using coulometric sensor,” In Annual Book of ASTM Standards. ASTM Philadelphia, pp. 532-537, 1995.